Achieving white light emission and increased magnetic anisotropy by transition metal substitution in functional materials based on dinuclear DyIII(4-pyridone)[MIII(CN)6]3− (M = Co, Rh) molecules
Wang, Junhao; Chorazy, Szymon; Nakabayashi, Koji; Sieklucka, Barbara; Ohkoshi, Shin-ichi; Journal of Materials Chemistry C 6 (2018) 473–; doi:10.1039/C7TC03963H

data_7236937
_publ_section_title
;
 Achieving white light emission and increased magnetic anisotropy by
 transition metal substitution in functional materials based on dinuclear
 DyIII(4-pyridone)[MIII(CN)6]3&#x2212; (M = Co, Rh) molecules
;
_journal_issue                   3
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              473
_journal_paper_doi               10.1039/C7TC03963H
_journal_volume                  6
_journal_year                    2018
_chemical_absolute_configuration unk
_chemical_formula_moiety         'C26 H26 Dy N10 O7 Rh, H2 O'
_chemical_formula_sum            'C26 H28 Dy N10 O8 Rh'
_chemical_formula_weight         873.99
_space_group_IT_number           36
_space_group_name_Hall           'C 2c -2'
_space_group_name_H-M_alt        'C m c 21'
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      36
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_space_group_name_H-M   'C m c 21'
_atom_sites_solution_hydrogens   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.3
_audit_creation_date             2017-04-23T19:31:02-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_audit_update_record
;
2017-08-30 deposited with the CCDC.
2017-11-18 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.8508(9)
_cell_length_b                   15.1527(10)
_cell_length_c                   14.0756(10)
_cell_measurement_reflns_used    24918
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      27.478
_cell_measurement_theta_min      3.054
_cell_measurement_wavelength     0.71075
_cell_volume                     3167.4(4)
_computing_molecular_graphics    'Ortep for Windows (Farrugia, 2012)'
_computing_publication_material  'WinGX publication routines (Farrugia, 2012)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      90(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID'
_diffrn_measurement_method       \w
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0831
_diffrn_reflns_av_unetI/netI     0.0485
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            24918
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.478
_diffrn_reflns_theta_min         3.054
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.925
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.879
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR (Rigaku, 1995)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.833
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1716
_exptl_crystal_preparation       'Magnetic properties,Luminescent'
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.136
_refine_diff_density_min         -2.379
_refine_diff_density_rms         0.141
_refine_ls_abs_structure_details
;
 Flack x determined using 1329 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.45(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.113
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     323
_refine_ls_number_reflns         3759
_refine_ls_number_restraints     122
_refine_ls_restrained_S_all      1.101
_refine_ls_R_factor_all          0.0542
_refine_ls_R_factor_gt           0.0456
_refine_ls_shift/su_max          0.02
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0129P)^2^+25.7197P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.067
_refine_ls_wR_factor_ref         0.0689
_reflns_Friedel_coverage         0.921
_reflns_Friedel_fraction_full    0.999
_reflns_Friedel_fraction_max     0.999
_reflns_number_gt                3407
_reflns_number_total             3759
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7tc03963h2.cif
_cod_data_source_block           shelx_CCDC1
_cod_database_code               7236937
_shelx_estimated_absorpt_t_min   0.735
_shelx_estimated_absorpt_t_max   0.755